TECHNICAL INFORMATION ON BUILDING MATERIALS TIBM - 32 FOR UfSE IN THE DESIGN OF LOW-COST HOUSING
THE NATIONAL BUREAU OF STANDARDS UNITED STATES DEPARTMENT OF COMMERCE WASHINGTON, D. C.
August 29, 1936
PAINT PIGMENTS— YELLOW, . BROWN, BLUE, GREEN, AND BRONZE
This is urimarily^a digest of the sections of Bureau of Standards Circular No, o9> "Paint and Varnish", (November 17, 1917),'*' and Tech- nologic Paper No. 274, "Use of United States Government Suecif ication Paints and Faint Materials", (December 15, 1924), ^ Ly p, H. Walker and
E. F. Hickson, dealing with general composition , characteristics, and uses of yellow, brown, blue, green, and bronze pigments.
The following papers contain additional information relative to paint pigments, oil paints, and water paints:
TIBM - 30 "Paint Pigments—White" TIBM - 31 "Paint Pigments—Black, Red, and Lakes"
TIBM - 33 "Federal Specification . Paint Pigments and Mixing Formulas" TIM - 3U "Federal Specification Ready-Mixed Paints, Semi- paste Paints and Mixing Formulas’"' TIBM - 35 "Preparation of Paints from Paste and Dry Pigments" TIBM - 36 "Preparation of Paints from Semipaste Paints, Thinning Ready-Mixed Paints, and Preparation of Water Paints" TIBM - 43 "Aluminum Paints"
Pigments are "the fine solid warticles used in the preparation of paint, and substantially insoluble in the vehicle, "3 In general, it may be
^Out of print. May be consulted in Government depositor}*- libraries.
p Available from Superintendent of Documents, Government Printing Office, Washington, D. C. .(Price 10 cents).
^Qpioted from "Standard Definitions of Terms Relating to Paint
'Specifications", American Society for Testing Materials ( 1 93 3 )
’ • • -• •• PP. 735-73 9 .
031736-C - 1 - assumed that pigments composed of very fine particles, having high re- fractive indices, provide the greatest covering power and opacity.
Federal Specifications are specifications adopted hy the Federal Speci- fications Executive Committee and approved hy the Director of Procure- ment, Treasury Department, for use of all departments and establishments of the Federal Government.^
Yellow Pigments— Chrome Yellow
General Composition and Types ; Chrome yellows are compounds of lead with chromic acid.
Chrome Yellow Medium is a nearly pure lead chromate.
Chrome Yellow Light , Lem on, or Canary contain a considerable amount of lead sulphate or other insoluble, lead salt, intimately mixed with lead chromate,
Chr ome Yell 6w Q range is a basic chromate precipitated from alkaline solutions, ranging in color from pale orange to almost scarlet.
Characteristics : Chrome yellows range in color from deep orange to light yellow. They are colors of . considerable brilliance, good color strength and hiding power, fairly durable but slowly affected by atmospheric conditions. Sulphides turn them black. Hence, ultramarine blue contain- ing sulphide must not be mixed with them. They cannot be used with silicate of soda, lime, or other alkaline substances as such substances turn them to an orange or red color.
Federal Specification : "Chrome Yellow; Paste-In-Japan See TT-C-291 , Dry, , | Paste- In-Oil (Lemon, Medium, Orange)."
Zinc Chromate and Barium Chromate
Characteristics : Doth zinc and barium chromate are light yellow in color, quite permanent., but lower in color strength and hiding power than lead chromate. The zinc chrome is not a pure chromate, but appears to be a double salt.
Use: Their use in paints is limited because of cost, although at the present time, the use of zinc chrome in rust inhibitive priming paints for metal is growing.
Copies of all Federal Specifications mentioned in this digest may be obtained from Superintendent of Documents, Government Printing Office, Washington, D. C. (Price 5 cents each).
- 2 - .
General Composition : Yellow ochers are natural earths containing hydrated oxide of iron (linonite, SFegO^^l^O) as the coloring matter. Various ochers contain 10 to 60 percent hydrated oxide, -the remainder being siliceous matter or clay.
Characteristics and Grades : In color they vary from pale yellow (citron) to very dark, almost olive. When of good quality, yellow ochers are ex- cellent uigments, are permanent in color, and work well with all vehicles and other pigments. With white thev produce fine cream or "buff tints. They are used primarily as a tinting color.
French ocher is the "best grade. English ocher is darker in color. American ochers range from those that are fairly good, though lacking in ouacity, "brightness, tinting -power, and freedom from grit, to those that are simply mud. Golden ocher is ocher- strengthened in color and given a ' r ellow tone through the addition of chrome yellow, which fades after a time, leaving only the natural ocher effect.
Federal : Sueoification See TT-0-111, "Ocher; Fry, Paste-In-Japan , and Paste-In-Oil 11
General Composition : Raw siennas resemble yellow ocher in general composition, being earthy substances colored by hydrated iron oxide. There is usually a little manganese oxide present. Rest grades are known as "Italian siennas".
Characteristics : Raw siennas are brownish yellow in color, and more transuarent than the yellow ochers. With white they produce beautiful cream tints which have greater color strength than ochers.
Use: Raw siennas are invaluable as staining and graining colors. They are -undesirable for body colors.
Yellow Oxide of Iron
Production : Yellow oxide of iron is produced on a large scale by precipitating a solution of ferrous sulphate with lime or soda ash, and then oxidizing the ferrous hvdroxide by aerating it with hot air.
Characteristics : It is uniform, very soft in texture, and possesses a tinting strength which is several times greater than that of yellow ocher. It contains about 90 percent ferric hydroxide.
Use : Yellow oxide of iron, at the present time, is used extensively as a staining and tinting pigment. It is also used largely in enamels,, particularly those of the synthetic rosin type.
-3 - Cadmium Yellow
Character! -sties. and Use :- Cadmium yellow is a sulphide of cadmium, used in enamels. It is also prepared as cadmium lithopones, which are cheaper than the pure cadmium sulphide.
Han sa Yellow
Characteristics .and Use : Hansa yellow is an organic, yellow pigment dye. It is the most permanent yellow pigment on exposure to sunlight. Although very expensive, it is used_ to some extent in Yellow lacquers and syn- thetic enamels.
Brown Pigments—Burnt Sienna
Production and Color ; Burnt sienna is uroduced by calcining raw sienna which changes its color to an orange red or subdued red "brown of great richness.
11 Kinds : "House Painters Bu rnt Sienna is strong in coloring matter, opaque, and is intended to serve as a tinting color. "Grainers 1 Burnt Sienna" is chosen for its transparency, richness, clearness, and is used as a body color (characteristic cherry), especially in graining. It is also used extensively for producing the conventional mahogany, in which case, it is generally strengthened in reddish tone by adding rose pinlc or
'' similar red colors. -
General Composition : Paw umber is a natural earth pigment, similar in composition to the siennas but containing considerable amounts of manganese .oxide. Best grades, known as "Turkey umber", come from Cyprus.
Characteristics and Use ; Raw umber has a yellowish brown color with an olive tone. It is permanent, mixes well with vehicles, is of medium opacity, and fair strength. It gives drab tints with white, and a great variety of other tints when mixed with colored pigments, for which purpose it is extensively used.
General Composition : Burnt umber is calcined raw umber.
Characteristics : It has a rich brown color, which, while darker than raw umber, should be free from redness.
Use: Burnt umber is used for the. -same purpose as raw umber. However, the tints formed are of a different 'order of drab.
- U - . ,
Metallic Sr owns or Mineral Browns
Pro Inc t ion and Colors : Metallic ‘browns or mineral "browns are uroduced from native ores which, iroon roasting, develou colors ranging from "bright red "brown to dark -on role
Charac teri stic s : They are ouaoue fairly -permanent, changing "but little , on exposure and can "be mixed with other uigments with good results.
Use : Such "browns are extensively used to uaint roofs, barns, iron bridges, and similar surfaces where a good substantial covering is reouired without much regard for beauty of finish.
Vandyke Brown (Cassel Earth or Cologne Earth)
C-eneral Composition : Vandyke brown is a uigment of carbonaceous character usually found in or near bogs.
Characteristics and Use : This pigment is soluble in dilute alkali, forming a solution which may be applied to wood and ureciuitated in the grain with dilute acid giving a very good and uermanent walnut stain. When ground in oil and thinned with turpentine, it makes a good walnut oil stain which is not too transuarent and is decidely uermanent. However, it does retard very strongly the drying of linseed oil.
" Sau brown 11 is a commercial dry soluble form of Vandyke brown.
The color of Vandyke browi may also be obtained by using burnt umber, drou black, and Prussian blue, producing a color that is per- manent, but lacking the transparency of true Vandyke brown.
Synthetic Brown Oxide of Iron
Production and Characteristics : Synthetic brown oxides of iron are very rich shades of brown uigments made synthetically from iron salts. They are uniform, soft in texture, very strong in tinting strength, and generally contain over 95 uercent oxides, of iron.
Blue Pigments—Prussian Blue
General Composition : Prussian blue is an oxidized ureciuitate uroduced by ureciui tating uotassium ferrocvanide with ferrous suluhate.
Characteristics and Use ; Prussian blue, which is a characteristic dark blue in color, is a transuarent uigment of great strength, 1 u'ound giving to a ton of white lead a decided sky blue tint. It is fairly permanent exceut in contact with alkalies or lime, which decolorize it rauidly. With white uigments it should give a decided blue tint, not uurulish or muddy. As Prussian blue is very fine in texture, it does not settle in the vehicle, and hence it is used as a dipuing paint.
Pederal ": Suecificatiori ' See TT-P-691, "Prussian-Blue; Dry, Paste-In-Japan Paste- In-Oil."
- 5 - . . "
Production : Ultramarine blue is produced artificially by heating' to- gether clay, silica, sodium carbonate, sodium sulphate, charcoal, rosin and sulphur. The resulting oroduct is then ground, roasted, and washed
Characteristics : In color this "pigment varies from a pure blue to colors "bordering on green (green ultramarine). It is bright but of low color strength. Although it is affected by weak acids, it is per- manent when exposed to sunlight, alkali, or lime. The sulphur in ultramarine darkens white lead carbonate ,. and discolors chrome yellow and other colors containing lead.
Use : Ultramarine blue is used largely in house -painting for mailing tints with zinc white.
Federal Spe ci ficat ion: See TT-U-^51. "Ultramarine-Blue; Dry, Paste- In-Japan, Paste-In-Oil .
General Composition : Cobalt blue is a compound of oxides of aluminum
and cobalt . . .
Characterist ics : It has a fine greenish blue color, -permanent to light, and is not affected by alkali, lime, or acid. It can be mixed with any other pigment or color. Because of the high price of genuine cobalt blue, the so-called commercial -product is a suitable ultramarine blue mixed with a little zinc white to .-provide a close imitation of cobalt blue
General Composition : Blue lead is essentially a basic lead sulphate’ with an excess of lead oxide mixed with varying small quantities of lead" sulphide , lead sulphite, zinc oxide, and carbon.
Characteristics : It is a dark blue-gray -pigment, affected by exposure to light which fact is of little importance as blue lead is not used for coloring power. After drying, when mixed as a paint, it is com- paratively immune against darkening by coal gas.
Use: Blue lead is used to a considerable extent as a protective coating for metallic surfaces.
Federal Specification : See TT-B-Ug6, "Blue-Lead; Basic-Sulphate, Dry
11 and Paste-In-,Oil . •
Characteristics and Use : Monastral blue is a new, blue pigment dye (copper phthalocvanine) that has appeared on the market, which gives a very beautiful, blue .tint. It appears- to be destined f-omuse as.' a’ g;
’ ! 1- pointing ink pigment. h :
- - -6 - s " s
'' jJi ' ( Green' Pfgmdhts—Chrome Green -
Production : Chrome green can' be made simply "by mixing together Prussian blue and Chrome yellow. However, in color works, the necessary solu- tions to produce both Prussian blue and chrome yellow are made up and then mixed together, the resulting chrome green being_a very intimate mixture of the blue and yellow.
Characteristics : In tone the mixtures range from very rale yellow green to a ver: r deep blue green. They have great covering power and good color strength, but are not very durable and are subject to the limitations' of both Prussian blue and chrome jrellow.
Common Grades and Use : "Commercial Greens" are composed of about 75 percent barvtes or silicate to 25 -percent color. As a body pigment, commercial greens answer very well. Pure Green known commercially as "chemically uure" is preferred for tinting purposes.
Federal Suecification : 3ee TT-C-236, "Chrome, Green; Pure, Pry, Paste- In-Japan, Paste-In-Oil .
Chrome Oxide Green
Grade : True Chrome Oxide Green is chromic oxide (CrpO^), a rather expensive, -permanent, dull color of satisfactory hiding- power. " C-uignets 1 Green" or "Viridian" is a carefully made product of the best grade, which is more or less hydrated and usually contains boric acid. "Chrome Ocher" is a clay stained with chromic oxide. It has little value.
Federal Suecifications : See TT-C-271, "Chrome ,’ Green ; Oxide."
General Composition and Use : Emerald green is -poisonous copper aceto- arsenite, known as "Paris Green", which is extensively used as an insecticide. Its use as a paint pigment has almost entirely ceased.
General Composition : Verdigris is a basic acetate of copper.
Characteristics : It possesses a pale bluish green color which is not permanent.
Use : Verdigris is used to some extent for decorative effects, and in marine paints as a protection against barnacles.
- 7 - s
. i ' ‘t i ^
Green Earth - (Terre Verte , or Verona Green)
General Composition ; The so-called' green eartlis are usually complex silicates of magriesium, or other ajlhali "base and ferrous iron.
Characteristic ; They are uermanent, semiopaque, and their colors are dull "bluish green varying to a "bluish gray.
" Use : Although their chief use is in disterrroer" (water paint), they are used somewhat by manufacturers of mixed paints to produce certain neutral greenish tints with white. A good quality of> green earth brightened with certain basic coal-tar dyes is used as a cheap lime- proof green color.
Metallic Pigments ("Bronzes)
Bronze Paints : Very finely divided metals or alloys are used in the so-called bronze uaints^
Aluminum Bronze is metallic aluminum.
Conner Bronz e is metallic copper.
Gold Bronze is the term applied to finely divided alloys of : copper, zinc, and tin which have colors resembling gold.
Bronze Powders generally contain small amounts of oil or fatty matter such as stearine. They may be dyed* with coal-tar dyes, resulting in brilliant reds, greens, blues, nurnles, etc. The dyed colors are not permanent on exposure to Sunlight.
Federal Specification : See TT-A-U76, "Aluminum-Powder; (For) Paints " (Aluminum-Bronze-Powder) »
- g -